Microstructure and Mechanical Behavior of High-Entropy Alloys Microstructure and Mechanical Behavior
Embed Size (px)
Transcript of Microstructure and Mechanical Behavior of High-Entropy Alloys Microstructure and Mechanical Behavior
Microstructure and Mechanical Behavior of High-Entropy Alloys
Joseph J. Licavoli, Michael C. Gao, John S. Sears, Paul D. Jablonski, and Jeffrey A. Hawk
(Submitted August 6, 2015; published online August 27, 2015)
High-entropy alloys (HEAs) have generated interest in recent years due to their unique positioning within the alloy world. By incorporating a number of elements in high proportion, usually of equal atomic percent, they have high configurational entropy, and thus, they hold the promise of interesting and useful properties such as enhanced strength and alloy stability. The present study investigates the mechanical behavior, fracture characteristics, and microstructure of two single-phase FCC HEAs CoCrFeNi and CoCrFeNiMn with some detailed attention given to melting, homogenization, and thermo-mechanical processing. Ingots approaching 8 kg in mass were made by vacuum induction melting to avoid the extrinsic factors inherent to small-scale laboratory button samples. A computationally based homogenization heat treatment was given to both alloys in order to eliminate any solidification segregation. The alloys were then fabricated in the usual way (forging, followed by hot rolling) with typical thermo-mechanical processing parameters em- ployed. Transmission electron microscopy was subsequently used to assess the single-phase nature of the alloys prior to mechanical testing. Tensile specimens (ASTM E8) were prepared with tensile mechanical properties obtained from room temperature through 800 �C. Material from the gage section of selected tensile specimens was extracted to document room and elevated temperature deformation within the HEAs. Fracture surfaces were also examined to note fracture failure modes. The tensile behavior and selected tensile properties were compared with results in the literature for similar alloys.
Keywords deformation, FCC crystal structure, fracture, high- entropy alloys, microstructure, tensile properties
Consider the design of an entirely new alloy. The first design input is always the desired properties defined by the target application. One may then go on to choose the crystal structure (e.g., FCC, BCC, etc.) that will impart the desired properties. The alloy may also be solid solution or precipitation strength- ened in which case compatible elemental additions and their effects can then be considered. For example, if a FCC solid solution strengthened alloy is the goal, per the Hume-Rothery rules, a list might be made of elements having a stable FCC matrix—Al, Ni, Cu, etc., as well as a list of elements that form FCC phase at some temperature (Fe, Co, etc.). However, this list may be misleading. For example, adding Al (FCC) to Fe stabilizes the BCC phase, while adding Mn (BCC) to Fe stabilizes the FCC phase. Thus, a more sophisticated approach is required such as the well-known CALPHAD method. The successful use of this method is highly dependent on the availability of accurate thermodynamic databases and must be coupled with experimental validation.
The application of the CALPHAD method in alloy design has led to significant departures from conventional composi- tions; but for both practical and historical reasons, most alloys are designed around one principal element. The supposition is that the principal element�s native structure will dominate the characteristics of the alloy leading to similar performance. Additional elements are then added to modify some combina- tion of physical and/or mechanical properties relevant to the alloy�s intended application. This may include phase stability, solid solution strengthening, and secondary phase formation. In this manner, classes of alloys have been developed around iron, aluminum, titanium, and nickel. While the number of com- mercially relevant alloys developed in this manner is large, designing an alloy around one element is restrictive. One rapidly expanding field of research is focused on designing alloys with multiple principle elements typically in equi-molar, or near equi-molar, concentrations (Ref 1, 2). These alloys have been designated high-entropy alloys (HEAs) (Ref 3).
Generally, HEAs are materials with at least five or more principal elements, and were so named because their mixing entropies in solution are much higher than alloys based on a single element. Some alloys with
phases that can form when multiple elements exist together in high concentrations. More importantly, a highly disordered solid solution imparts appealing properties that are typically not observed in traditional alloys. For example, HEA properties may include high room temperature strength/hardness, good wear resistance, good high temperature strength, good struc- tural stability, and good corrosion/oxidation resistance (Ref 1). While these properties appear promising, many studies were carried out utilizing small-scale melting techniques, and therefore, the observed properties may not translate directly upon scale up when the same compositions are produced via commercial methods.
The performance levels thatmay be achieved froman alloy are highly sensitive to processing history. Within the HEA literature, there have been limited investigations on the importance of melt processing, homogenization heat treatment, and thermo-me- chanical processing. Kao et al. (Ref 5) studied the microstructure and mechanical properties of AlxCoCrFeNi in the as-cast, ‘‘homogenized’’ (so-called, since no criteria for the homoge- nization cycle used was given), and mechanically deformed states. Zhang et al. subsequently examined the effect of annealing on the microstructure and properties of CoCrFeNiCuAl (Ref 6) and CoCrFeNiTiAlx (Ref 7). Ng et al. used a series of thermo- mechanical treatments to study the stability of the solid solution phases in a high-entropy Al0.5CoCrCuFeNi and found that the solid solution phases were stable only at high temperatures >850 �C and at temperatures below 300 �C (Ref 8). Most HEA studies present properties for thematerial in the as-cast condition. In this state, the dendritic structures that result from non- consumable arc melting (i.e., button) dominate performance. Finally, many small-scale melts only allow for compression samples to be produced as opposed toASTMstandard size tensile specimens. The limited geometric sample size has forced comparisons between HEA compression tests and commercial alloy tensile tests which may be misrepresentative (Ref 9).
Non-consumable arc melting is useful for making small- scale trial heats of material for laboratory investigations. However, this approach has many technical issues that can potentially influence the characteristics of the resulting alloy. A close look at non-consumable arc melting is needed to understand these limitations. Consider a non-consumable arc melted ingot. Such ingots are produced in contact with a water- cooled copper hearth. The hearth cools the ingot such that it is never fully molten, and as such, this melting technique makes it highly improbable, if not impossible, to fully and completely mix the elemental constituents in the alloy. Differences in density and melting point of the elements tend to exacerbate this problem with high density, high melting point elements such as W, Ta, and Nb being particularly hard to incorporate into a non-consumable arc melted ingot.
A solidification artifact also arises from this approach. Typically, an ingot made in this way results in an erratic dendrite structure that forms during the solidification process. If the portion of the alloy ingot in contact with the copper hearth melts, it solidifies nearly instantaneously forming a ‘‘chill grain’’ region which is free of dendrites. Quite often, the bottom of the ingot is not completely melted and displays character- istics of a heat-affected zone found in weldments (which is effectively what a non-consumable arc melted ingot is). Meanwhile, those regions near the upper surface, and topmost sides, solidify into long columnar dendrite grains with orien- tations dependent on both hearth configuration (i.e., the direction of heat extraction) and melt practice (i.e., heat input).
Furthermore, the inevitable shrink cavity is difficult to control and may, or may not, have connectivity to the surface. Thus, the structure of the ingot, and presumably the physical and mechanical properties are complex, difficult to describe, and vary throughout the ingot, as well as from ingot to ingot. As a result of these melt-solidification artifacts along with other considerations, non-consumable arc melting is not used to produce alloys on an industrial scale because they may produce non-representative and non-reproducible properties. The HEAs produced and reported herein were made by conventional vacuum induction melting (VIM), which is a commercial type process often used to produce industrial scale ingots.
The alloys investigated in this effort represent well-reported, single-phase HEAs of CoCrFeNi and CoCrFeMnNi. Previous results in the literature on similar HEAs (Ref 10-13) do not provide much information related to the effects of ingot size and thermo-mechanical processing on the chemistry, microstructure, and mechanical properties. This report focuses on NETL�s efforts to produce single-phase HEAs of kilogram size using commercial melting, thermo-mechanical processing, and heat treatment practices. The results of the melting campaign are provided through analysis of microstructure and mechanical behavior at various temperatures.
2. Experimental Procedures
2.1 Alloy Manufacture and Heat Treatment
Two alloys with nominal compositions CoCrFeNi (desig- nated as HEA1) and CoCrFeMnNi (designated as HEA2) were melted using VIM. Each VIM furnace charge weighed approx- imately 7.8 kg and was composed of feed